1 I ~~AGARD.P9 ADISR GR RE Mi AGARD CONFERENCE PROCEEDINGS NO. 98 Specialists Meeting on Stress Corrosion Testing Methods V%$ b'60d o tv NORHA'TADIS TRiBUTION NDAVILABIOLT ON BACK COVER N;ATIONAL TECHNICAI
2 AGARD-CP-98 NORTH ATLANTIC TREATY ORGANIZATION ADVISORY GROUP FOR AEROSPACE RESEARCH AND DEVELOPMENT (ORGANISATION DU TRAITE DE L'ATLANTIQUE NORD) SPECIALISTS MEETING ON STRESS CORROSION TESTING METHODS Papers presented at the Structures and Matcriak Panel 33rd Me, tg 1ield aý Bitssels, Belgium, 5 and 0 Octo 1ei '71
3 THE MISSION OF AGARD The mission of AGAR. "; to bring togethier the leading personalities of the NATO nations in the fields of sciei-.zz?nd technology relating to aerospace for the following purpose-. - Exchanging of scientific and technical information; - Continuously stimulating advances in the aerospace sciences ieievant to strengthening the common defence posture. - Improving the co-operation among member rnations in aerospace research and development,, - Providing scientific and technical advice and assistance to the North Atlantic Military Committee in the field of aerospace research and development: Rendering scientific and technical ossistance. as requested, to other NATO bodies and to member nations in cor.neation with research and development problems in the aerospace field. - Providing assistance to member nations fo- the purpose of increasing their scientific and technical potential, - Recommending effective ways for the member nations to use their research and development capabilities for the commnn benefit of the NATO community. The highest authority within AGARD is the National Delegates Board consisting of officially appointed senior representatives frc,a each Member Nation. The mission of AGARD is carried out through the Panels which are composed for ey )erts appointed by the National Delegates, the Consultant and Exchange Program and.the Aerospace Applications S, -dies Program. The results of AGARD work are reported to the Member Nations and the NATO Authonties t',rough the AGARD series of publications of which this is one. Participation in AGARD activities is by invitation only and is normally limited to citizens of the NATO natioas. The material in this publication has been produced direclmy from copy supplied by each author. Publihhed January d bl Ie In hi, I dolti' and Rcjvo'P,'/!itmtI / lt bir/,ord flo, c. l Imr/,te' o t n,,it I ll/)
4 SYMPOSIUM CHAIRMAN Dr. A. M., Lovelace Director, Air Force Materials Laborato-y Wright-Patterson AFB Ohio, 45433, USA tft SYMPOSIUM VICE-CHAIRMAN MAY 2 17 Prof. Dr. Ing. F, Boi'lenrath L Institut fdr Werkstoffkunde -Q Rhein-Westf, Technirz.he Hochschal. Templergraben, Aachen, West Germany STRUCTURES AND MATERIALS PANEL Ct1AIRMAN Dr., A. J. Barrett Director, Eigineering Sciencc's Data Unit Royal Aeronautical Society Regent Stre(. London, W1R7AD, England COORDINATOR Dr. D.. E. Piper Staff Scientist Metallurgy & Composites Laboratory Lockheed Palo Alto Research Laboratory Lockheed Missiles & Space Company, Inc Hanover Street Palo Alto, California, 94304, USA PANEL EXECUTIVE Mr. Peter K. Bamberg AGARD ili
5 FOREWORD The problem of stress-corrosion cracking was identified by the Structures and Materials P-anel of AGARD as a major area of concern to the aerospace industry. A Working Group on Stress Co.'rosion Cracking was formed in 1965 with a basic objective _o evaluate and disseminate current knowledge about the phenomenon A Specialists meeting held in 1966 (recordtd in AGARD publication R-540)/1966 entitled "Corrosion ol Aircraft") and a Symposium held in Spring 1907 (AGARD publication CP-18/1967 entitled "Stress-Corroaion Cracking in Aircraft Structural Materials") attracted leading personalities of the NATO nations in the stress-corrosion field and resulted in the identification of two areas for further study:. 1. The need to survey and publish current knowledge about the engineering practices to avoid stress-corrosion cracking, and Z. The need to survey and publish current recommendations concerning a stand-rd method of test for stress-corrosion with particular emphasxsq on the generation of data significant to the designers of aerospace components. A survey of NATO countries carried out in 1968 (AGARD publication R-570/1969) and a Symposium held in Fall 1969 (AGARD publication CP-63/1969) have highlighted those engineering practices used to avoid streed-corrosion cracking. A similar survey conducted during 1969 (AGARD publication AR-25/1970) and a Specialists meeting on Stress-Corrosion Testing Methods convened during the 33rd Structures and Materials Panel Meeting in October 1971 (with proceedings published in this AGARD report) constitute the efforts of the Wowking Group toward the second assignment mentioned above. The program of this Specialists meeting on Stress-Corrosion Testing Methods was prepared to encourage discussion of (a) the utility and significance of stress-corrosion cracking data to current engineer ng and design practices, (b) the progress being made by NATO countries toward standardization of test techniques for stress-corrosion cracking, and (c) those test methods which might be recommended as standard techniquec in the immediate future. Another importrnt purpose of the meeting was to bring together those key personnel from North America and Europe who are striving on a voluntary basis to fo,'mulate standard methods and recommended practices for stress -corrosion testing. It is expected that the meeting will stimulate the interchange of information concerning such techniques ana eventually lead to joint participation in any cooperative testing programs planned as a result of the meetin g. The opening lectire introduces the types and quality of data which are useful in design analysis and the following five papers describe the activities and attitudes of the various corrosion and fracture committees in the United States and Europe toward standardization of testing methods. The next contribution summarizes the proceedings of the recent NATO Sc ence Committee Conference (April, 1971) on Theory of Stress Corrosion Cracking of Alloys with special reference to testing methods, The remaining invited papers were solicited on the basis that they provided new information about stresscorrosion cracking in general and/or stress-corrosion testing methods in particular.
6 CONTENTS Reference ENGINEERING UTILITY AND SIGNIFICANCE OF STRESS CORROSION CRACKING DATA by W. E Anderson 1 PROGRESS TOWARD STANDARDIZATION OF SCC TEST TECHNIQUES BY THE AMERICAN SOCIETY FOR TESTING AND MATERIALS by H. Lee Craig, Jr. 2 PROGRESS TOWARD STANDARDIZATION OF SCC TEST TECHNIQUES BY THE NATIONAL ASSOCIATION OF CORROSION ENGINEERS AND THE ALUMINUM ASSOCIATION by D. 0. Sprowls 3 STRESS CORROSION TEST METHODS - THE EUROPEAN FEDERATION OF CORROSION CONTRIBUTION by R. N., Parkins 4 SOME IMPORTANT CONSIDERATIONS IN THE DEVELOPMENT OF STRESS CORROSION CRACKING TEST METHODS by R, P. Wei, S. At. Novak, and D. P, Williams 5 CURRENT PROGRESS IN THE COLLABORATIVE TESTING PROGRAMME OF THE STRESS CORROSION CRACKING (FRACTURE MECHANICS) WORKING GROUP by A. H. Priest and P. McIntyre 6 THE SCIENCE COMMITTEE CONFERENCE ON THE THEORY OF STFFSS CORROSION CRACKING OF ALLOYS by J. C. Scully 7 MEASURING THE DEGREE OF CONJOINT ACTION BETWEEN STRESS AND CORROSION IN STRESS CORROSION by F. H. Cocks 8 ph AND POTENTIAL MEASUREMENTS DURING STRESS CORROSION OF ALUMJNUM ALLOYS by J. A. Davis 9 STRESS CORROSION TESTING OF WELDED JOINTS by T. G., Gooch 10 SCREENING TESTS OF SUSCEPTIBILITY TO STRESS CORROSION CRACKING by G. J, Biefer ana J., G Garrison 11 STRESS CORROSION TESTING OF TITANIUM ALLOYS by S. J, Ketcham, C., E., Neu, and S. Goldberg 12 FACTORS INFLUENCING STRESS INTENSITY VALUES AND CRACK PROPAGATION R,ýTES DURING STRESS CORROSION CRACKING TESTS OF HIGH STRENGTH STEELS by A., H, Priest and P., McIntyre 13 AN APPARATUS FOR STRESS-CORROSION TESTING WITH LARGE PRECRACKED WOL SPECIMENS by L. J., Ceschini and W., G.. Clark, Jr. 14 TENSILE-LIGAMENT INSTABILITY AND THE GROWTH OF STRESS CORROSIC I CRACKS IN A HOMOGENEOUS Zn-Mg-Cu ALUMINUM ALLOY by J., H., Mulherin 15 AN ULTRAHIGH VACUUM SYSTEM FOR DETERMINING TH"' EFFECTS OF GASEOUS ENVIRONMENTS ON FATIGUE AND FRACTURE PROPERTIES OF METALS by H., L. Marcus and P. J., Stocker 16 ACOUSTIC EMISSIONS AND SLOW CRACK GROW1H IN HIGH STRENGTH F CEEL by R. W. Staehle and G., E. Kerns 17 A CONTRIBUTION TO STRESS CORROSION TESTING O1 ALUMINUM ALLOYS by G. Bollam 18 V
7 INFLUENCE OF TEST METHOD ON STRESS-CORROSION BEHAVIOR OF ALUMINUM ALLOYS IN SEA WATER Reference by G. J. Danek 19 DISCUSSION OF PAPER ENTITLED INFLUENCE OF TES!. METHOD ON STRESS CORIuSION BFHAVIOR OF ALUMINUM ALLOYS IN SEA WATER (PAPER 19) by D. 0. Sprowls and J. G. Kaufman PARTICIPATION A L'ETUDE DE LA CORROSION SOUS TENSION DE CERTAINS ALLIAGES D'ALUMINIUM A HAUTE RESISTANCE par R. Doste 20 RESULTS OF COMPARATIVE STRESS-CORROSION TESTS ON Al-Zn-Mg-Cu ALLOYS USING DIFFERENT TYPES OF SPECIMENS by W. Lehmann 21 STRESS CORROSION CRACKING OF MARTENSITIC PRECIPITATION HARDENING STAINLESS STEELS by M. Henthorne 22 INVESTIGATION OF AN ACCELERATED STRESS CORROSION CRACKING METHOD by M. Hugo, J., Bellot, and E. Herzog 23 MICROSCOPIC IDENTIFICATION OF STRESS-CORROSION CRACKING IN STEELS WITH HIGH YIELD STRENGTH by E. H., Phelps 24 HOT SALT STRESS CORROSION CRACKING OF TITANIUM ALLOYS-OVERVIEW AND IMPACT ON SPACE SHUTTLE APPLICATION by W B. Lisagor and J. E., Gardner 25 THE USE OF SLOW Sxi.AIN-RATE EXPERIMENTS IN EVALUATING RESISTANCE TO ENVIRONMENTAL CRACKPTG bj J., E. Reinoehl and W. K. Boyd 26 EXPERIMENTAL TECHNIQUES USED ro STUDY STRESS COIROSION MECHANISMS IN AIRCRAFT STRUCTURAL ALLOYS by G. M. Hoch, W. E. Krupp, and K., E. Weber 27 FRACTURE INITIATION P.ND STRESS CORROSION CRACKING OF WELDED JOINTS OF ALPHA- TYPE TITANIUM ALLOYS by C. Chassain and P, R, Krahe 28 PRELIMINARY REPORT ON RESEARCH ON THE INFLUENCE OF THERMOMECHANICAL TREATMENTS ON STRESS CORROSION CRACKING BEHAVIOR O0- AISI 4340 STEEL by R. DeSantis, L. Mattt.)li, and T. Songa 29 PRELIMINARY RESULTS OF MECHANICAL AND STRESS-CORROSION TESTS ON PLATES OF 7075 ALLOY PRODUCED BY A NEW PROCESSING TECHNIQUE by E. DiRusso, M. C.nserva, and M., Buratti 30 WRITTEN DISCUSSIONS OF PAPERS PRESENTED AT MEETING 1 19A Page v vi v,
8 ENGINEERING UTILITY AND SIGNIFICANCE OF STRESS CORROSION CRACKING DATA W. E. Anderson BATTELLE PACIFIC NORTHWEST LABORATORIES Richland, Washington USA
9 yi SUMMARY An engineering design analyst traces throu',h some historical experiences with cracking and fracture problems to indicate the significance of corrosion acting that cracks concomitantly develop either with stress. in "open" These or "closed" experiences areas; suggest i.e., a either des,.:-;tion at regions accessible to the ambient environment and direct view, or, at regions which are st-ucturally hidden. These latter regions can be thought of as "nooks and crannies" having the same geometric nature as cracks or crevices. Stress corrosion cracking is, first, a geometric disruption of the affected material; e.g., by fretting, mechanical damage like nicks and scratches, :orrosion pits and internal fissures or cavities. Then follows an expansion of the disrupted region into the form of a crack, and, subsequent enlargement of the crack border. Useful tests and evaluation methods now exist for the structurally "open" problems;, this permits reasonable estimation of crack enlargement rates and hence service performance for short-lived components under simple loading and environmental experiences. Similarly credible tests and methods for longer-lived items or the structurally "closed" problems seem not yet in hand, even for the most elementary loading and environmental sequencing. Such problems presently defy practical prediction. Lots of low-cost, moderately accurate data from many sources appears to have more utility for the analyst than limited araounts of very specific data. Specimen configurations and methods suitable for low-cost testing are examined and "new" possibilities suggested.
10 1-1 ENGINEERING UTILITY AND SIGNIFICANCE OF STRESS CORROSION CRACKING DATA W. E. Anderson INTRODUCTION Iy "landmark" experience with ambient-environment airframe stress-corrosion cracking (SCC) care about in the late '50's as a result of a broken landing gear beam on a transport-type aircraft. Figure 1 shows the broken beam; Figure 2, the fracture face region. The break occurred at night, while the airplane was quiescent, having been refueled a little earlie,', prior to en intended early morning flight to the customer. Rain had been tflling for about two hours; thf first in more than two weeks. Review of the craft's operations showed that it had been in lightweight,lying status, but that a flat tire had been experienced two weeks previously and iý was changed on the field runway. There seemed to be no question as to the initiating structural defect. "he locally dented tube broke srom the inside first, developing an effective crack length of about two wall-thicknesses prior to the "wetting" experience. The fracture toughness of this material was estimated at Gc 105 lb/:,i., whence, for the final crack length indicated by the change in rusting, the local bending stress figured at about 50,000 psi. A check with the geometry and load conditions at the time provided verification of this estimate. The timing of this event was important; we had been accumulating confidence in the crack-strengthanalysis methods of Irwin and Kies (1), who had visited the company on occasion. Our work was initially centered on the danaged-fuselage problem (2), but the principles seemed generally useful for,,u6i of the high-strength aircraft structure. Relevance to fatigue crack propagation occurred to Paris in 1957 (3) and soon enough data was accumulated from new tests reported in the literatute (4-7) to permit evaluation of the scheme; it turned out that crack extension rate per cycle was correlated very nicely on the basis of the elastic stress Field parameter, K, but it was to be some time before we could get the idea into published form (8 and 9). We recognized the potential effects of envronmental influences on cracking (10), and by the April 1959 meeting on stress corrosion in Pittsburgh. we.,ere throughly ready to "see" the significance of wedging-type corrosion products on SCC behavior described by Nielsen (11). Meanwhile, we had been struggling with the "thickness effect" on toughness of cracked aluminum structures (12 and 13) and possible metallurgical influences or. cracking resistance generally (14 and 15). There was a lot to do. Sometime earlier we had been having troubles with,igh strength steels and "static fatigue." The conditions behind the 1954 summary of B-36 (Figure 3) experiences by Sachs (16) probably influenced thinking generally toward some method for steel protection which didn't cause more trouble than it cured. Among other means (like painting) there was developed a "porous cadmium plating" as a consequence of undesignated nocturnal urea addition to a plating sulution. The porous plating would indeed permit the baking-out of hydrogen at low temperatures. After a number of uneasy service difficulties, however, it became brutally clear that oxide of hydrngen could reenter the "pores" and serve as a very efficient electrolyte for the cadmium-steel "battery" at each interface-deep pore. The behavior was so regular that we could place a wet cotton wad on a strip so plated and, under a particular bending strain, could predict its early failure time much too accurately ( a' had them breaking at 30 min. - 5 min.). The "fix" was to fill the pores with a polymer. Zoeller and Cohen (17) showed some of these structural aluminum and stee. stress corrosion cracking problems, several of their figures are reproduced here (see Figures 4, 5 and 6). EARLY EXPERIENCES THE HISTORICAL PERSPECTIVE These modern difficulties took on a different perspective when, in 1963, I was piv,.aged to explore the older engineering journals at Lehigh University. Along with some remarkcble descri~tions of early American steamboating boiler explosions (one of wh.ch, by Ewbank (18) in 1843, seems likly to have involved stress corrosion cracking of copper), there was reported in 1844 by one John M. Batchelde- the "Explosion of Hardened Steel" (19). His experience is portrayed in Figure 7, which he explains this way, "...The cause of the fracture is. probably, the same as observed in the glass toy called Prince RuIert's drops, made by pouring melted glass into cold water; the outside is suddenly contracted, while the nart~cles in the interior, cooling more gradually, assume a differpit crystaline form, and burst asunder a, soon as the cohesion of the external coating is destroyd.". ",iew his remuarks as showing marvelous insight. Water storage tanks of iron and steel seemed susceptible to unexpected failur s unoer.luiescent f' nditions; let me mention a few. The tank containing water from "...the silvery Tded... wh,." hurst in 1867 (20) was possibly due to stress-corrosion aggravated cracking. So alsc, c.ight ha e.,o " 14, June 29, 1881 water tank failure at Cincinnati (21)., One episode in the rather droll accou-,t oc this event is rendered in Figure 8. Perhaps the 1904 early morning failure of the wate, tank at Sanford, Maine, stewed from such crack aggravating causes, too (22). I shall not deny that triggering mechanisms for such accidents ray iave included temperature-differential stressing between the relatively warm interior and coldish outside winds, but the influencing factor of corroined stress and corrosion effects is difficult to discard entirely. It is even more difficult to find any other reason but stress corrosion for the unfortuoate cause of failure in the second attempt to span the St. Lawrence River with a "Quebec Bridge." The dramatic sequence of events is pictured in Figure 9. The truss was lo.t because a cast steel support rocker broke unexpectedly under perfectly quiescent conditions; a view of the rocker region is shown in Fiqure 10. (Reference 23)
11 * 1-2 There were problems with unexiected fractures of manganese bronze and tobin bronze bolts in the same time period; one was at the Panama Canal (24). An imaginary rendering of this difficulty is given in Figure 11; what else but stress-corrosion' The residual stresses in ordance and helmets of WWI vintage caused rather inusual spontaneous fractures; these were mentioned by Howe and Groesbeck in 1920 (25). An attempt at picturing the problem is shown in Figure 12. During lunch break in a 1934 German construction shop, a freshly cut beam split open; Campus showed a picture of this event (26), and it is reproduced hare as Figure "13. Can these crackithg mechanisms be anything but concomitant action of stress and environment? How shall all these incidents and acctdei.,s be described? What rationale might explain their precise atomic-level mechanisms? These problems are clearly important to the structural designer and he must include them in his considerations. But how? To this observer there are two classes of cracxing problems depicted in these historical events. One is cracking of "open" regions and the other is a class of structurally "closed" regions. Whether the distinction is fundamental or trivial seems not yet clear. But from this point of view it is easy for me to appreciate the 1930 remarks on corrosion in aircraft by Rawdcn (27)(referencing U.R. Evans' 1927 papers on the subject), who pointed out that the rate of corrosion in a crevice "...on the basis of an oxygen concentration-cell is often very much greater than elsewhere on the same structure..." RECENT AEROSPACE EXPERIENCES Aircraft and their engines in 1930 may have been somewhat less structurally complex than those of today, but the SCC problem certainly din't lessen with the increased complexity! Outtweiler (28) has provided an example of elevated temperature stress corrosion in titanium alloy. Originally blamed oi fretting alone (Figure 14), the test disc (Figure 15) caused the spin-pit mess shown in Figure 16. It was later found that there was deposition of silver along with the fretting shown at the hole, and the assigned cause was stress corrosion. Typical structural problems in transport aviation were kindly outlined by Weesner (29) in connection with another work. Figures are taken from his offerings. All are traced to stress corrosion as the initiating or crack-extending phase of these service problems with modern turbine-powered airframes. Other survey work within the tnduqtry (30) indicated that the corrosion problem in civil aircraft generally was not astonishingly more severe in overwater operations than overland operations; these figures, then may be considered "typi'cal" examples. A summary to this point must recognize clear evidence of concern by aircraft structural designers, manufacturers and operators for the very real rroblem of stress corrosion cracking. Review of the figures presented suggests classification of the experiences into "open" problems, where the influencing environment can readily reach the affected area, and into "closed" problems where the cracking is initially "hidden" by fasteners and faying surfaces of other structural components. Two of the documented cases reproduced here were obviously associated with fretting as the causative factor in geometric disruption of the affected material surface. The writer interjects personal views he believes are correct that other forms of disruption are similarly effective, e.g. corrosion pits, intermetallics, atomic structure voids and plain old mechanical damage. Furthermore, the view is held that if either the stress or the causative environment were absent from the affected region, the cracking process would be significantly retarded or altogether voidr-. ACTUAL CONDITIONS AND THE TESTS WE USE TO MODEL THEM AN UPPER WING SKIN An example of the structural loads experience of an airplane component may help point out what I regard as real-life complexity of the SCC problem. Consider a certain portion of the upper wing skin on a conventional civil transport aircraft. Figure 27 depicts an "average" day's experience; it is important to note that about two-thirds of the load-time history is tensile. Local residual stresses, somewhere in this region, may very well be nearly at yield. As the nominal stress level fluctuates from positive to negative, it can be assumed that this local region will experience the same range of fluctuations, but with an elevated mean. A simplified representation, in real time, of the diurnal loads experience is shown in Figure 28. Loth the nominal stresses at some region and the likely stresses at some other (residually stressed) region, ave depicted as the approximated service cycles occur. This representation is probably the most elementary form of stress corrosion load-time cycling which would be credible to design analysts like me. It appears I shall have to resort to ad hoc approximations of the "worst likely" services experiences until something along the lines of "Miner's Law" is established for SCC., I am heartened at the progress along these lines (31 and 32). (he loading problem of Figure 28 emphasizes to me the need for Lonsidering the conjoint action of SCC and fatigue. I know that fatigue cracks as small as 0.1 mm seem to behavw as the larger ones when they are defined by the stress field parameter concept (33), and providing the plastic zone ;urrounding th 2crack border is small compared to the minor crack dimension. If the residual stress maximum of 440 in/m is considered in this light, the case of a crack 0.1 mm deep is associated with a plastic zone only a fqw times smaller than the crack depth. However, for the nominal condition of a stress maximum at 125 MN/mS, the plastic zone ii about 1/40 the minor crack dimension of 10 4 m. But whether these cracks might or might not behave in a manner describcd by the stress-fieid-parameters concept, they are real problems because defects like intermetallics as well as mecnanical damage or corrosion pits 0.1 mm deep may occasionally be found, It is clear that concern for their effects on structure needs careful attention, Figure 29 is presented at a scale of interest. The stress corrosion cracking data are from Hyatt (34), and the fatigue cracking rates are estimated from the literature for the short-transverse grain direction,
12 Both conditions are assumed to be "worst-like'iy a rcumstances which might arise in civil transport service. At the nominal condition, maximm Ki N0m" 3 ý1, and the 7079-T651 short-transverse plate exhibits stress corrosion cracking rates of 10-5 a sec; about 1 mm per dayl If the condition of 8.8 M.Um-3/ arose, the cracking rate could exceed one ililimetter per hauri On the basis of five cycles per day, the cracking (due to cycling loads only) might range from about 10-3 noday to some very much lower value. Using this comparison then, it can be seen that mechanical cycling alone is several orders of magnitude less serious than the worst stress corrosion cracking. What is not clear is how the two might interact if the two conditions were to be imposed simultaneou-ly, as they could very well be in practice. Consideration of the upper wing skin example should demonstrate that not only is it important to have a measure of static-load stress-corrosion cracking resistance, but also it is necessary to have an evaluation of the combined effects of load-cyclinq and environment. In the present case, the other realities of temperature and pressure have not been implicated. At some tink these must be considered as pat of the total environmental and load sequencing variations. From the sheer inmensity of this problem it is Easy to appreciate why civil aircraft designers make very real attempts to provide structures that can safely contain large amounts of cracking damage. Before continuing to specific specimen testing remarks, consider Figure 29 again. Two other abscissa scales besides cracking rates in millimeters are shown. The aluminum unit cell is considered to be alout 4 A across, and requires the separation of three atomic bonds per unit cell for complete fracture (if the process can be averaged for one unit cell thickness). At the lower stress-corro*jon cracking rates of a few unit cells per second or slower, each atom has the opportunity to vibrate 1011 or more times before a bond is broken. As the cracking speeds reach that of brittle fracture, the atoms have the chance for only about one vibration before breaking apart. This kind of information is not only interesting to me, but I feel I gain some "perspective" from it. TESTS Conventional SCC test methods have not correlated well with actual cracking behavior of structures. For example, conventional testing (Figure 30)(35) failed to identify the unusual cracking rates of 7079 aluminum alloy. Is it possible that the SCC crack tip is sometimes blunted? That's suggested by Figure 31, from Creager and Paris (36), who referenced Mulherin's work. However, regardless of the details, the dominant message of experl~nce is that SCC testing must take on broader dimensions than the important but incomplete story told by 600 seconds of immersion in 3.5% NaCl solution followed by 3000 seconds out of it. Harking back to the upper wing skin and the stress history of Figure 27, one of the most apparent needs is for tests which include various cycles of hold-time. The results of some of our own experimentation in this area are shown in Figures 32a and 32b (37). Altogether the combined fatigue and environment effects may be described as shown in Figure 33. It appears that some materials behave as "A", and others as "B". Perhaps this generalization is broadly true and perhaps some of you can say why and under what conditions the observed behavior will occur. But to get quantitative behavior numerous experiments are needed to find which are the "A's" and which are the "B's". We are trying to make these "timed-hold" tests in the simplest, least costly but credibhe apparatus we can conjure up. At the present time our cycling hydraulics (38) are off-the-shelf items arranged as shown in Figure 34. TEST SPECIMENS Part of the course in "new" SCC developments may be guided by the specimen configuration. Different specimens can provide different kinds of useful data. Smith and Piper (39) summarized many of these, Figure 35; for some of these, the crack-tip stress field intensity varies with crack length as shown in Figures 36 and 37. There are at least two additional specimen types which may prove of value in SCC testing, tigure 38; they cause variation with crack length as shown. All the selected examles are compared in Figure 39. Both the ring specimen and (certain configurations of) the wedge-loaded ce,;ter-hole specimen have the interesting property of an increasing, then decreasing, crack-tip stress field as the c.rack extends. Such behavior may be particularly useful for obtaining several items of crack-resisting data fiom one test. This possibility is illustrated in Figure NEW TEST SPECIMENS Between the foregoing several specimen types there may be sufficient diversity to meet most practical problems of SCC material testing. However, further refinements for structural testing can be suggested. An adaptation of the center-hole rectangular-perimeter design is illustrated in Figuro 41. Pressing the boundaries of this specimen will cause the hole wall to yield in compression. Following load removal, the yielded region will be in residual tension. The specimen is now self-stressed, and may be subjected to appropriate environments. Building on this approach, representative faying materials and fasteners may be affixed to provide representative crevices. This scheme might prove well-suited to temperature and pressure cycling patterns of real aircraft structures., Taie s;ccimens are inexpensive and can be destructively sectioned as needed. With just a little more imagination we can doubtless "invent" otl-!r tests that are both inexpensive and credible to the likes of me., There is still a lot to do. CONCLUDING REMARKS The problem of SCC in aircraft structures has been reviewed, as I see it, using an historical approach that I have found helpful. The important point is that SCC problems are stitl very much with us, and the!1
13 1-4 total *ecology of the crack" is a very comp'ex Inter-relationsh'p betweea loads, load-cycles, chemical interactions of the structure with the environment, and normally occurring abuse in service. I have intended to point up the need for further attention to realistic mode.ing of the complex parameters affecting real structures in the tests we choose to apply to materials. I,, this respect, we have come full cycle to a remurn to the original sense of the word *test", which means to abuse a material or structure sufficiently well that its satisfactory behavior means we can use it for its intended purpose with con- "fidence that it ui," perform its function safely and economically. The essential contributions of pnysicists, metallurgists, and chemists and the crucial contrlbutions of traditional testing must continue. These contr- ions have been and will surely remain invaluable. However, I believe there is a trend toward more complete modeling of actual service conditions in SCC testing, and I look forward with great hope and anticipation to substantial orogress in coping with these failure.qechanisms over the next decade. It r;stresses me to think that I might someday become a victim of SCC and have to petition a city, somewhare, to get back nl fee for a car wash, like Mr. Reid of Seattle (Figure 42)(43). REFERENCES 1. J.A. Kies and G.R. Irwin, "Fracturing and Fracture Mechanics," Welding Research Supplement, Feb A. Sorensen, "Some Design Considerations for Tear-Resistant Airplane Structures," las Meeting, Jan. 23, P.C. Paris, "A Note on Variables Effecting the Rate of Crack Growth Due to Cyclic Loading," Addendum N, , , The B:)elng Company. 4. W. Weibull, "The Propagation of Fatigue Cracks in Light-Alloy Plates," SAAB TN 25, W. Weibull, "Effect of Crack Length and Stress Amplitudes on Growth of Fatigue Cracks," Men. 65, Aero Res. Inst. of Sweden, D.E. Martin and G.M. Sinclair, "Crack Propagation Under Repeated Loading," Proc. Third US Cong. Appl. Mech., June A.J. McEvily, Jr. and W. 111g, "'ilhe Rate of Fatigue-Crack Propagation in Two Aluminum Alloys," NACA TN 4394, Sept P.C. Paris, M.P. Gomez, and W.E. Andersun, "A Rational Analytic Theory of Fatigue," The Trend in Engineering, Vol. 13, No. 1, Jan D. R... Donaldson and W.E. Anderson, "Crack Propagation Behavior of Some Airframe Materials," Crack Propa- 4ation Symposium, Cranfleld, England, Rei 4, p W.E. Anderson in discussion of N.A. Nielsen, "The Role of Corrosion Products in Crack Propagation In Austenitic Stainless Steel. Electron Microscopic Studies," Physical Metallurgy of Stress Corrosion Fracture, Metallurgical Society Conferences, Vol. 4, 1959, pp. 147 and P.C. Paris and W.E. Anderson, "On the Brittle Fracture of Structures," The Trend in Engineering, University of Washington, Vol. 12, No. 2, April W.E. Anderson and P.C. Paris, "Evaluation of Aircraft Material by Fracture," Metals Engineerin., Quarterly, Vol. 1, No. 2, May 1"'. pp W.L. Anderson, Patent No. 3,284,194, Aluminum Alloy (with W.E. Quist) assignors to the Boeing Co., D.E. Piper, W.E. Quist, and W.E. Anderson, "Tte Effect of Composition on the Fracture Properties of 7178-T6 Aluminum Alloy Sheet," Met. Soc. Conf., Vol. 31, AIME, G. Sachs, Survey of Low-Allo Aircraft Steels Heat-Treated to High Strength Levels, WADC TR , Dept. of Comm. PB 1R1667, 19b H.W. Zoeller and B. Cohen, "Shot Peening for Resistance to St'ess-Corrosion Cracking," Metals Engineering Quarterly, Feb T. Ewbank, J. Franklin Inst., 3rd Series, Vol. V, 1843, p J. 1. Batchelder, J. Franklin Inst., 3rd Series, Vol. VIII, 1844, p "Bursting of a Reservoir at Kelso," Engineering, (London), Vol. 4, Dec., 20, 1867, p "An Accident at Cincinnati," Engineering News, Vol., 8, July 9, 1881, p C.W. Sherman, "A Standpipe Failure at Sanford, Me.," nineering News, Vol. 52, Dec. 1, 1904, p H. Barker, "Quebec Bridge Suspended Span Falls Into River in Hoisting," Engineering News, Vol. 76, Sept. 14, 1916, pp S...
14 24. "Nore Evidence of Unreliability of the Stronger Bronzes," Engineering News, Vol. 76, Nov. 23, 1916, H.N. Howe and E.C. Groesbeck, Trans. Am. Inst. of Mn. and Netall. Enars., Vol. 62, 1920, p F. Campus, in Residual Stresses and Metal Constrction, anetals Ed. W.R. Osgood, Reinhold, N.Y., k7. H.S. Rewdon, "Corrosion Prevention Mlethods as Applied in Aircraft Construction", Proc. ASTM, Vol. 30, Part 11, 1930, pp Letter to R.E. Duttwetler, Evendale Works, from Schenectady Laboratory, General El ectric Co., August 29, 19E Letter from J. Weesner, Pan American World Airways to W.E. Anderson, Feb. 24, P.C. Johnson, American Airlines, Enclosure #3 to Ref R.P. Wei and J.D. Landes, "Correlation Between Sustained-Load and Fatigue Crack Growth in High Strength Steels," Materials Research and Standards, Vol. 9, 1969, pp , 44 and J.K. Barsom, "Corrosion-Fatigue Crack Propagation Below Kjscc," Engineering Fracture Mechanics, Vol. 3, No. 1, 1971, pp J. Schijve, "Significance of Fatigue Cracks in Micro-Range and Macro-Range," Fatigue Crack Propagation - ASTM STP-415, 1967, pp M.V. Hyatt, "Use of Precrdcked Specimens in Stress Corrosion Testing of High Strength Aluminum Alloys," Corrosion, Vol. 26, No. 11, Nov. 1970, pp D.O. Sprowls, "Reporting and Evaluating Stress Corrosion Data," Stress Corrosion Testing, ASTM STP-425, 1966, pp M. Creager and P.C. Paris, "Elastic Field Equations for Blunt Cracks with Reference to Stress Corrosion Cracking," International Journal of Fracture Mechanics, Vol. 3, No. 4, Dec. 1967, pp F.R. Vollert, F.J. Lewis and W.E. Anderson, "Expluratory Cracking-Rate Studies with Aluminum Alloy T6 in Wet and Dry Air Under Triangular and Trapezoidal Cyclic-Load Wave Forms," Battelle-Northwest,3NWL-SA-3270, March F.J. Lewis, F.R. Vollert and W.E. Anderson, "An Inexpensive Electro-Hydraulic Cyclic-Load Test System," Battelle-Northwest BNWL-SA-3182, March H.R. Smith and D.E. Piper, "Stress-Corrosion Testing with Precracked Specimens," The Boeing Co. D , ARPA #878, June W.F. Brown, Jr., and J.E. Srawley, "Plane Strain Crack Toughness Testing of High Strength Metallic Materials," ASTM STP-410, J.C. Newman, Jr., "An Improved Method of Collocation for the Stress Analysis of Cracked Plates with Various Shaped Boundaries," NASA TN D-6376, August J.P. Gallagher, "Experimentally Determined Stress Intensity Factors for Several Contoured Double Cantilever Beam Specimens," Engineering Fractnre Mechanics, Vol. 3, No. 1, July 1971, pp "WHAT HAS 4 WHEELS, 2 EYES AND CAN'T SEE? "-e of the smallest dollar-amount ordinanres to clear through City Council for many years was a recer, claim payment for $2.25 to reinmurse Floyd H. Reid, th Ave. N.W., for a car wash. Reid was driving past a city sewer-pumping truck in Elliott Avenue West when "something broke" and his car was deluged with mud. "It was just like someone tossing a blanket over the car," Reid said." The Seattle Times, Washington, Nov. 6, 1966.
15 1-6 FIGURE 1. FRACTURED LANDING GEAR FIGURE 2. FRACTURE AREA OF FAILED LANDING GEAR EQUALIZER WALKING BEAM EQUALIZER P IN SELF-ALIGNING FIXED-LINK BEARING OLEO-STRUT FIGURE 3. PROBLEMS WITH HIGH-STRENGTH STEEL, 1954(16)
16 * 1-7 Landag pvar mob of Impi "7.T94 rinel. *AWNe dms~mujnd Idng WS arms Amw. d"u skew e mos.h w 9'11.:aA. In~~~o F IGURE 5. CRACKING IN LADAG GE FTNGEA gnalnafmofca" (7079-T6AD17 kw ATvtoinge ftum hmirg tcrickl in ~teinsiou l mar graam. Crack Is trunnone fitting of 433CM steel (220 to 240 km.). FIGURE 6. CRACKING IN A 4330M STEEL TRUNNION FITrING( 17 )
17 1-8 COOLED STORED CUT C oo HEATED (21. ONE HOUR LATER FIGURE 7. A MARTENS ITIC PRINCE RUPERT'S DROP( 19 ) FIGURE 8. THE CINCINNATI FLUSH (1881)(21).1 (,
18 L1 1-9 FIGURE9. FAILUJRE OF THEQUEBEC BRIDGE(3 FIGURE 10. SUPPORT ROCKER FROM QUEBEC BRIDGE; BEFORE AND AFTER ( 23 )
19 - -. ~.~ FIGURE 11. BRONZE COUNTERWEIGHT ASSEMBLY BOLT FAILURE, PANAMA ( 24 ) C'-4 Lffor FIGURE 12. THE HELMET WAR (1920); VOLUTE CRACK ING( 25 )
20 FIGURE 14. FRETTING AT A BOLT HOLE (Ti ALLOY)(28 FIGURE 13. FAILURE OF A STEEL I-BEAM' 6 lrom FIGURE 15. RECONSTRUCTION OF AFAILED FIGURE 16. SPIN-PIT FOLLOWING FAILU'RE Ti DISC ( 28 )